Designation: D5873 − 05
Standard Test Method for
Determination of Rock Hardness by Rebound Hammer Method1 This standard is issued under the ﬁxed designation D5873; the number immediately following the designation indicates the year of original origin al adoption or, in the case of revis revision, ion, the year of last revision. revision. A number in paren parenthese thesess indicates the year of last reappr reapproval. oval. A superscript epsilon (´) indicates an editorial change since the last revision or reapproval.
1. Sco Scope* pe*
Specimens and Verify Specimens erifying ing Confo Conformance rmance to Dimens Dimensional ional and Shape Tolerances D4879 G D4879 Guid uidee for Geo Geotech technic nical al Map Mappin ping g of Lar Large ge Und Under er-ground Openings in Rock D7012 Test Method for Compressive Strength and Elastic D7012 Moduli Mod uli of Int Intact act Roc Rock k Cor Coree Spe Specim cimens ens und under er Vary arying ing States of Stress and Temperatures 2.2 ISRM Standards: Suggested Method for Determination of Schmidt Rebound Suggested Hardness3 Suggested Method for Quantitative Description of Discontinuities in Rock Masses3
1.1 This test method covers covers the testing apparatus, apparatus, sampling, sampling, test specimen preparation, and testing procedures for determining the reb reboun ound d har hardne dness ss num number ber of roc rock k mate material rial using a spring-driven steel hammer, referred to variously as a rebound hammer, impact test hammer, or concrete test hammer. 1.2 Thi Thiss test method method is bes bestt sui suited ted for roc rock k mate materia riall with uniaxi uni axial al com compre pressi ssive ve str streng engths ths (se (seee Test Met Method hod D7012) D7012) ranging between approximately 1 and 100 MPa. 1.3 1. 3 Th Thee po port rtab able le tes testin ting g ap appa para ratu tuss ma may y be us used ed in th thee laboratory or ﬁeld to provide a means of rapid assessment of rock hardness or to serve as an indicator of rock hardness.
1.4 The values values stated in SI uni units ts are to be reg regard arded ed as the standard.
3.1 For common deﬁnitions deﬁnitions of terms in this standa standard, rd, refer to Terminology D653 Terminology D653..
1.5 This standar standard d doe doess not purport purport to add addre ress ss all of the safet sa fetyy co conc ncer erns ns,, if an anyy, as asso socia ciate ted d wi with th its us use. e. It is th thee responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use.
3.2 Deﬁnitions of Terms Speciﬁc to This Standard: 3.2.1 rebound hammer— a portable, spring loaded, pistontype, steel hammer used to classify the hardness of rock in the ﬁeld or laboratory. 3.2.2 rebound hardness number— HR, a dimensionless number representing empirically determined, relative hardness of rock roc k mate materia riall or oth other er har hard d sub substa stance nce by use of a reb reboun ound d hammer.
2. Referenc Referenced ed Documents Documents 2.1 ASTM Standards:2 C805 Test C805 Test Method for Rebound Number of Hardened Concrete D420 Guide D420 Guide to Site Characterization for Engineering Design and Construction Purposes D653 Termino erminology logy Relating to Soil, Rock, and Contained Fluids D3740 Practic Practicee for Minimu Minimum m Requir Requirements ements for Agencies Engaged in Testing and/or Inspection of Soil and Rock as Used in Engineering Design and Construction D4543 Practices D4543 Practices for Preparing Rock Core as Cylindrical Test
4. Signi Signiﬁcanc ﬁcancee and Use 4.1 The reb reboun ound d har hardne dness ss meth method od pro provid vides es a mea means ns for rapid classiﬁcation of the hardness of rock during site characterization for engineering, design, and construction purposes (see Guide D420 Guide D420)), geotechnical mapping of large underground openings in rock (see Guide D4879 D4879), ), or reporting the physical descri des cripti ption on of roc rock k cor coree (se (seee Pra Practic cticee D4543) D4543). The rebound hardness number, H r , can serve in a var variety iety of eng engine ineerin ering g applica app licatio tions ns tha thatt req requir uiree cha charac racter terizat ization ion of roc rock k mate materia rial. l. These The se app applica licatio tions ns incl include ude,, for exa exampl mples, es, the pre predic diction tion of penetration penetr ation rates for tunnel borin boring g machin machines, es, determ determination ination of rock roc k qua quality lity for con constr struct uction ion pur purpos poses, es, and pre predic diction tion of hydraulic erodibility of rock.
This test method is under the jurisdiction jurisdiction of ASTM Committee D18 Committee D18 on on Soil and Rock and is the direct responsibility of Subcommittee D18.12 D18.12 on on Rock Mechanics. Current edition approved Nov. 1, 2005. Published November 2005. Originally approved in 1995. Last previous edition approved in 2005 as D5873 – 00(2005)e1. DOI: 10.1520/D5873-05. 2 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected]
For Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website.
3 Brown, E. T., ed., Suggested Methods: Rock Characterization, Testing, and Monitoring, International Society of Rock Mechanics: Pergamon Press, London, 1981.
*A Summary of Changes section appears at the end of this standard Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959. United States
Copyright by ASTM Int'l (all rights reserved);
D5873 − 05 4.2 This test method is of limited use on very soft rock or very hard rock (unconﬁned compressive strengths less than approximately 1 MPa or greater than 100 MPa).
only by repeated, heavy blows with a geological hammer and cannot be scratched with a common 20d steel nail. 7. Specimen Preparation
4.3 The results of this test method are not intended for conversion to strength data suitable for design.
7.1 For a block or core specimen, determine its length by taking the average of four lengths measured at four equally spaced points on the circumference and record to the nearest 5 mm.
NOTE 1—Several types of rebound hammers are commercially available to accommodate testing of various sizes and types of concrete construction (See Test Method C805) and rock material. NOTE 2—The quality of the result produced by this standard is dependent on the competence of the personnel performing it, and the suitability of the equipment and facilities used. Agencies that meet the criteria of Practice D3740 are generally considered capable of competent and objective testing and sampling. Users of this standard are cautioned that compliance with Practice D3740 does not in itself assure reliable results. Reliable results depend on many factors; Practice D3740 provides a means of evaluating some of those factors.
7.2 For a block or core specimen, determine its diameter by taking the average of two diameters measured at right angles to each other approximately midway along the length of the specimen and record to the nearest 5 mm. 7.3 Report the moisture condition of the block or specimen. 7.4 The test surface of all specimens, either in the laboratory or in the ﬁeld, shall be smooth to the touch and free of joints, fractures, or other obvious localized discontinuities to a depth of at least 6 cm. In situ rock shall be ﬂat and free of surface grit over the area covered by the plunger. If the surface of the test area is heavily textured, grind it smooth with the abrasive stone described in 5.4.
5. Apparatus 5.1 Rebound Hammer, consisting of a spring-loaded piston, or hammer, which is projected against a metal anvil in contact with the rock surface. The hammer must travel with a ﬁxed and reproducible velocity. The rebound distance of the piston from the steel plunger is measured in a linear scale attached to the frame of the instrument and is taken as an empirical measure of rock hardness.
8. Calibration 8.1 Prior to each testing sequence, calibrate the hammer using a calibration test anvil supplied by the manufacturer for that purpose. 8.1.1 Place the calibration anvil in the core holder and conduct ten readings on the anvil. 8.1.2 Calculate the correction factor by dividing the manufacturer’s standard hardness value for the anvil by the average of the ten readings taken on the anvil.
5.2 Steel Base— A steel base of minimum mass of 20 kg to which specimens are securely fastened. Rock core specimens may be tested in a steel cradle with a semicylindrical machined slot of the same radius as the core, or ﬁrmly seated in a steel V-block, see Suggested Method for Determination of Schmidt Rebound Hardness. 5.3 Calibration Anvil— The standard calibration block used to calibrate the rebound hammer.
NOTE 3—If the instrument reads lower than the manufacturer’s standard hardness value, the correction factor will be greater than unity. If the readings are higher, the correction factor will be less than unity. NOTE 4—Operation of the rebound hammer is satisfactory if the calibration readings fall within the range provided by the manufacturer. If the calibration readings fall outside this range, the instrument must be cleaned, adjusted, or returned to the manufacturer for correction. NOTE 5—Rebound hammers require periodic servicing and veriﬁcation to provide reliable results.
5.4 Abrasive Stone— A medium-grained texture silicon carbide or equivalent material. 6. Sampling 6.1 Drill core specimens shall be NX or larger core of at least 15 cm in length. Block specimens shall have edge lengths of at least 15 cm. Rock surfaces tested in place, including natural outcrops or prepared surfaces such as tunnel walls or ﬂoors, shall have a smooth, ﬂat test area at least 15 cm in diameter.
9. Procedure 9.1 Place the steel base on a ﬂat, level surface that provides ﬁrm, rigid support, such as a concrete ﬂoor. 9.2 Securely clamp rock core specimens in a steel cradle with a semicylindrical machined slot of the same radius as the core, or ﬁrmly seat into a steel V-shaped block. Securely clamp block specimens to the rigid steel base in such a manner as to prevent vibration and movement of the specimen during the test.
6.2 Samples shall be representative of the rock to be studied. Obtain samples by direct sampling of subsurface rock units with core borings or by sampling blocks of rock material from outcrops that correlate with the subsurface rock unit of interest. At surface outcrops, avoid sampling and testing rock material weakened by weathering or alteration or is otherwise unrepresentative of the rock material of interest, see Suggested Method for Quantitative Description of Discontinuities in Rock Masses.
9.3 For tests conducted on specimens in the laboratory, orient the instrument within 5° of vertical with the bottom of the piston at right angles to and in ﬁrm contact with the surface of the test specimen. A guide may be used to ensure the rebound hammer is positioned for optimum performance. Position the hammer not less than one diameter from the edge of the specimen.
6.3 The rebound hammer is generally unsuitable for very soft or very hard rock. Conduct simple ﬁeld tests to quickly assess a rock material’s suitability for the rebound hammer test method. Scratch very soft rock with a ﬁngernail and peel with a pocket knife. An intact specimen of very hard rock breaks Copyright by ASTM Int'l (all rights reserved);
9.4 For tests conducted in situ on a rock mass, the rebound hammer can be used at any desired orientation provided the 2
D5873 − 05 plunger strikes perpendicular to the surface tested. The results are corrected to a horizontal or vertical position using the correction curves provided by the manufacturer.
more than seven units and determine the average of the remaining readings. To calculate the rebound hardness number ( H R) of the tested rock material, multiply this average by the correction factor determined in 8.1.2 and record the results to the nearest whole number.
9.5 Before conducting the tests, ensure the hammer is at the same temperature as the test specimens by exposing it to the ambient environmental conditions of the test area (indoors or outdoors) for at least 2 h.
11. Report 11.1 Report the following minimum information for each specimen or test area: 11.1.1 Source of samples, including geographic location; boring number, depth, orientation, and stationing; and rock type, 11.1.2 Weathering and alteration condition of samples, particularly when sampling a surface outcrop, 11.1.3 Type of specimen (core, block, or in situ); size and shape of specimen; and, if block type, whether cut or blasted, 11.1.4 Date of sampling and date of testing, 11.1.5 Storage conditions of samples (for example, exposure to temperature extremes, air drying, and moisture changes), 11.1.6 Type and model number of hammer, 11.1.7 Orientation of the plunger axis during the test, 11.1.8 Method of securing the sample (for example, V-block, or clamps), 11.1.9 Number of tests conducted, 11.1.10 Temperature of site at time of test, and 11.1.11 The individual and average values of hammer rebound, the value of the correction factor, and the rebound hardness number, H R (obtained in 10.1).
9.6 Compress the hammer spring by gradually depressing the plunger until the hammer is triggered and impact occurs. 9.7 Read and record the height of the plunger rebound to the nearest whole number, as measured on an arbitrary scale of 10 to 100 divisions located on the side of the hammer, before restoring the piston to its original extension. Repeat this procedure at ten representative locations on the specimen. Test locations shall be separated by at least the diameter of the piston and only one test may be taken at any one point. 9.8 If a specimen breaks during rebound testing, energy is absorbed during breakage and, consequently, the rebound reading will be lower than had it not broken. Any individual impact test that causes cracking or any other visible failure shall cause that test and the specimen to be rejected. 9.9 Some factors that may affect the results of the test include: 9.9.1 Rock at 0° C or less may exhibit very high rebound values. 9.9.2 Temperature of the rebound hammer itself may affect the rebound number. The hammer and materials to be tested should be at the same temperature. 9.9.3 For readings to be compared, the direction of impact, horizontal, upward, downward, and so forth, must be the same. 9.9.4 Different hammers of the same nominal design may give rebound numbers differing from one to three units and therefore, tests should be made with the same hammer in order to compare results. If more than one hammer is to be used, a sufficient number of tests must be made on typical rock surfaces to determine the magnitude of the differences to be expected.
12. Precision and Bias 12.1 Precision— No data exist to determine the precision of this test method in determining rock hardness. 12.2 Bias— There is no accepted standard value for H R for any material, therefore bias cannot be determined.
10.1 Using the data from the ten readings obtained in 9.7, discard readings differing from the average of ten readings by
13.1 core; hardness; rock mass; rock; unconﬁned compressive strength
Copyright by ASTM Int'l (all rights reserved);
D5873 − 05 SUMMARY OF CHANGES In accordance with Committee D18 policy, this section identiﬁes the location of changes to this standard since the last edition (00(2005)) that may impact the use of the standard. (1) Deleted Test Method D2938 in Sections 1.2 and 2.1, and replaced with Test Method D7012. ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (www.astm.org). Permission rights to photocopy the standard may also be secured from the ASTM website (www.astm.org/ COPYRIGHT/).
Copyright by ASTM Int'l (all rights reserved);